Download presentation

Presentation is loading. Please wait.

Published byKayli Ask Modified over 2 years ago

1
First Principles Calculations of PtN and MAX phases Sanjay V. Khare Department of Physics and Astonomy University of Toledo Ohio 43606 http://www.physics.utoledo.edu/~khare/

2
Outline Experiment on PtN PtN calculations About MAX phases MAX phases - calculations Conclusions

3
Experimental synthesis of PtN Experimental Synthesis and characterization of a binary noble metal nitride E. Gregoryanz, C. Sanloup, M. Somayazulu, J. Badro, G. Giquet, H-K. Mao, and R. J. Hemley, Nat. Mat. 3, 294 (2004). Although numerous metals react with nitrogen there are no known binary nitrides of the noble metals. We report the discovery and characterization of platinum nitride (PtN), the first binary nitride of the noble metals group. This compound can be formed above 45–50 GPa and temperatures exceeding 2,000 K, and is stable after quenching to room pressure and temperature. It is characterized by a very high Raman-scattering cross-section with easily observed second and third-order Raman bands. Synchrotron X-ray diffraction shows that the new phase is cubic with a remarkably high bulk modulus of 372(±5)GPa.

4
Structure of experimental PtN Data is taken from two samples once with N as the pressure medium and once with He as the pressure medium. All patterns at different pressure are consistent (see Fig. 3) and PtN can be indexed as f.c.c. (a = 4.8041(2) Å at 0.1 MPa) at all pressures. Although the Rietveld refinement is complicated by the strong Pt signal, the refinement agrees with the non-centrosymmetric space group F4–3m,to which the zinc-blende structure belongs,as well as the rock-salt structure (Fm3–m); the large mass difference between Pt and N makes it impossible to distinguish between these two structures from the diffraction intensities. The rock-salt structure does not have a first-order Raman spectrum and can therefore be ruled out. The zinc-blende structure has two Raman active peaks, consistent with the two strong first-order bands observed (see Fig. 1).

5
X-ray diffraction of PtN Figure 3 In situ X-ray diffraction data. a, X-ray spectra of PtN taken at different pressures.At ambient pressure the spectrum was taken with wavelength λ= 0.3311 Å and others with λ=0.3738 Å. Red crosses: data; green line: GSAS fit.b, Zinc-blende structure of PtN.c, Section of the CCD image at 28 GPa showing the powder-like texture; the asterisk indicates a rhenium diffraction ring. d, Detail of the inner section of the charged-coupled device image (shown in c) at ambient pressure with the arrow pointing at one of the two weak rings in addition to Pt and PtN signal.

6
PtN stoichiometry and back-scattered electron image

7
Forms of PtN in our study Zinc Blende Rock Salt Pt:N ratio 1:1 in all forms Face centered Cooperite Orthorhombic (PtS form)

8
Ab initio method details LDA, Ceperley-Alder exchange-correlation functional as parameterized by Perdew and Zunger Used the VASP code with generalized ultra-soft Vanderbilt pseudo-potentials and plane wave basis set Bulk supercell approach with periodic boundary conditions in all three dimensions Cut-offs of 224 eV for PtN, 300 eV for MAX phases, dense k- point meshes Forces converged till < 0.03 eV/ Å Used AMD Athlon dual processors at UT and OSC

9
Lattice constants for zb and rs forms of PtN Theory with VASP Zinc Blende Rock Salt a = 0.4699 nm (LDA) a = 0.4407 nm (LDA) 0.4781 nm (GGA) 0.4504 nm (GGA) B = 230 GPa (LDA) B = 284 GPa (LDA) 192 GPa (GGA) 226 GPa (GGA) Experiment, Gregoryanz et al. Nat. Mat. 3, 294 (2004) a = 0.4801nm B = 372 GPa

10
No effect of N vacancies on bulk modulus of PtN Theory with VASP Zinc Blende Rock Salt No significant change in bulk modulus was found by introducing vacancies. We used Pt 1 N 1-x, where x = 0, 0.037, and 0.125. Use 2 x 2 x 2 or 3 x 3x 3 fcc supercells. In experiment, of Gregoryanz et al. Nat. Mat. 3, 294 (2004) 0 < x < 0.05.

11
Elastic constants Elastic constants in GPa and stability If C 11 – C 12 unstable form. Also, any C ij unstable form. Also other conditions. Only stable form = rock salt.

12
Earlier theoretical work on PtN Theory with WIEN2K, Sahu et al., PRB 71, R041101 (2005). Zinc Blende Rock Salt a = 0.4804 nm (GGA) a = 0.4518 nm (GGA) B = 371 GPa (GGA) 431 GPa (GGA) Experiment, Gregoryanz et al. Nat. Mat. 3, 294 (2004) a = 0.4801nm B = 372 GPa Theory matches perfectly with experiment!

13
Our manuscript would have read like this We have done first principles calculations for the newly reported noble metal nitride PtN. Our calculations contradict experimental findings published in Nature Materials by a well known group. Our calculations also contradict theoretical findings by another well known theoretical group published in PRB Rap. Comms. We think we are right. Please accept this manuscript for publication.

14
More of earlier theoretical results for PtN Experiment, Gregoryanz et al. Nat. Mat. 3, 294 (2004) a = 0.4801nm and B = 372 GPa [8] B. R. Sahu and L. Kleinman, Phys. Rev. B 71, R041101 (2005). [9] R. Yu and X. F. Zhang, Appl. Phys. Lett. 86, 121913 (2005).

15
Summary of theoretical results for PtN

16
Some evolution of the other theory Erratum by B. R. Sahu et al., PRB 72, 119901 (E) (2005).

17
Conclusions of work on PtN 1.Zinc blende structure for PtN as claimed in experiment and an earlier theory is incorrect 2.There exists a stable form of PtN the rock salt phase. It is not superhard. Has B < 300 GPa. Its lattice constant is around 0.44 nm. 3. The experimental form of PtN remains unknown. 4. Published theory and experiment can match each other and both be self-consistently wrong!

18
What are MAX Phases? M = transition metal = A = A-group element = X = C or N = Electrically and thermally conductive materials Relatively soft Resistant to Thermal Shock Damage Tolerant Z M is the internal degree of freedom within the unit cell *M.W. Barsoum, Prog. Sol. Stat. Chem. 28 (2000) 201. HEXAGONAL MAX 211 PHASE M n+1 AX n (n=1,2,3) ZMZM

19
Atoms in unit cell P Q R P Q R are three sites in hcp packing. P X R M Q A R M P X Q M R A Q M

20
Barsoum’s Table *M.W. Barsoum, Prog. Sol. Stat. Chem. 28 (2000) 201.

21
Lattice constants and B for M 2 GaN, M = Ti, V, Cr

22
DOS Results for M 2 GaN, M = Ti, V, Cr

23
LDOS Results for M 2 GaN, M = Ti, V, Cr

24
Lattice constants and B for M 2 TlC, M = Ti, Hf, Zr B values lowest of all MAX phases studied so far.

25
DOS Results for M 2 TlC, M = Ti, Zr, Hf

26
LDOS Results for M 2 TlC, M = Ti, Zr, Hf

27
Conclusions of work on MAX phases 1.Calculated lattice constants and bulk moduli of Ti 2 GaN, V 2 GaN, and Cr 2 GaN. 2.Calculated lattice constants and bulk moduli of Ti 2 TlC, Zr 2 TlC, and Hf 2 TlC. 3.Calculated LDOS and DOS of Ti 2 GaN, V 2 GaN, and Cr 2 GaN. 4.Calculated LDOS and DOS of Ti 2 TlC, Zr 2 TlC, and Hf 2 TlC. 5.All six MAX phases are conducting. The M-A bonds are weaker than the M-X bonds. 6. Ti 2 TlC, Zr 2 TlC, and Hf 2 TlC have the lowest bulk moduli of all MAX phases studied to date.

28
Collaborators Senior J. K. Bording (Brookhaven National Laboratory) S. Kodambaka (T. J. Watson Research Center, IBM) B. R. Tuttle (Penn. State. Erie Campus) Students S. K. R. Patil (Mechanical and Industrial Engineering, U. of Toledo) J. A. Warner (REU at U. of Toledo 2005, U. of Wisconsin)

29
Institutional Support University of Toledo URAF Summer Fellowship Start up money University of Toledo University of Toledo parallel computing cluster Ohio Supercomputer cluster NSF REU program at University of Toledo

30
Thank you!

31
Raman spectra

Similar presentations

OK

DFT evolutionary search for Mg 2 Si under pressure Yu.V. Luniakov Institute of Automation and Control Processes, Vladivostok, Russia Department of Surface.

DFT evolutionary search for Mg 2 Si under pressure Yu.V. Luniakov Institute of Automation and Control Processes, Vladivostok, Russia Department of Surface.

© 2018 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

English 8 unit 12 read ppt on iphone Ppt on complex number for class 11 Ppt on human nutrition and digestion worksheet Ppt on product advertising definition Ppt on food supplements Ppt on windows 7 features Download ppt on turbo generator rotor Ppt on point contact diode picture Ppt on bmc remedy software Ppt on google products and services